Sequential structural transitions with distinct dielectric responses in a layered perovskite organic-inorganic hybrid material: [C4H9N]2[PbBr4].
Wang, Zhong-Xia; Liao, Wei-Qiang; Ye, Heng-Yun; Zhang, Yi; Dalton transactions (Cambridge, England : 2003) 44 (2015) 20406–20412; doi:10.1039/c5dt03277f

data_7037576
_publ_section_title
;
 Sequential structural transitions with distinct dielectric responses in a
 layered perovskite organic-inorganic hybrid material: [C4H9N]2[PbBr4].
;
_journal_issue                   47
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              20406
_journal_page_last               20412
_journal_paper_doi               10.1039/c5dt03277f
_journal_volume                  44
_journal_year                    2015
_chemical_formula_moiety         'Br4 Pb, 2(C2 H6 N), 4(C H3)'
_chemical_formula_sum            'C8 H24 Br4 N2 Pb'
_chemical_formula_weight         675.09
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-10-13 deposited with the CCDC.
2015-10-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 105.32(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.196(3)
_cell_length_b                   8.3416(17)
_cell_length_c                   8.2422(16)
_cell_measurement_reflns_used    0
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      -1.#IN
_cell_measurement_theta_min      -1.#IN
_cell_volume                     941.3(4)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku Mercury CCD'
_diffrn_measurement_method       \w
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1100
_diffrn_reflns_av_unetI/netI     0.1375
_diffrn_reflns_laue_measured_fraction_full 0.998
_diffrn_reflns_laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6231
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.477
_diffrn_reflns_theta_min         3.540
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    17.433
_exptl_absorpt_correction_T_max  0.031
_exptl_absorpt_correction_T_min  0.021
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'CrystalClear (Rigaku, 2005)'
_exptl_crystal_colour            pale-yellow
_exptl_crystal_density_diffrn    2.382
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             616.0
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         2.477
_refine_diff_density_min         -3.812
_refine_diff_density_rms         0.304
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.000
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     115
_refine_ls_number_reflns         2155
_refine_ls_number_restraints     103
_refine_ls_restrained_S_all      0.990
_refine_ls_R_factor_all          0.1144
_refine_ls_R_factor_gt           0.0668
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0423P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1288
_refine_ls_wR_factor_ref         0.1431
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1300
_reflns_number_total             2155
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt03277f2.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 
;
_cod_database_code               7037576
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              51852